On the pairwise cocrystallization of racemic compounds
Zhou, Fuli; Body, Carole; Robeyns, Koen; Leyssens, Tom; Shemchuk, Oleksii; CrystEngComm 25 (2023) 3060–3065; doi:10.1039/D3CE00226H

data_7246744
_publ_section_title
;
 On the pairwise cocrystallization of racemic compounds
;
_journal_issue                   20
_journal_name_full               CrystEngComm
_journal_page_first              3060
_journal_page_last               3065
_journal_paper_doi               10.1039/D3CE00226H
_journal_volume                  25
_journal_year                    2023
_chemical_formula_moiety         'C8 H14 N2 O2, C8 H7 Cl O3'
_chemical_formula_sum            'C16 H21 Cl N2 O5'
_chemical_formula_weight         356.80
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_Hall           '-P 1'
_space_group_name_H-M_alt        'P -1'
_atom_sites_solution_hydrogens   geom
_atom_sites_solution_primary     'dual space'
_audit_creation_method           SHELXL-2018/3
_audit_update_record
;
2023-03-09 deposited with the CCDC.	2023-04-28 downloaded from the CCDC.
;
_cell_angle_alpha                63.137(16)
_cell_angle_beta                 86.083(15)
_cell_angle_gamma                84.134(13)
_cell_formula_units_Z            2
_cell_length_a                   7.7370(14)
_cell_length_b                   10.7279(12)
_cell_length_c                   11.583(2)
_cell_measurement_reflns_used    3263
_cell_measurement_temperature    297(2)
_cell_measurement_theta_max      26.0970
_cell_measurement_theta_min      3.3200
_cell_volume                     852.9(3)
_computing_cell_refinement
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_data_collection       MAR
_computing_data_reduction
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
;
_computing_molecular_graphics    'MERCURY (Macrae et al., 2008)'
_computing_publication_material
;
'MERCURY (Macrae et al., 2008), Platon (Spek, 2009)'
;
_computing_structure_refinement  'SHELXL-2018/3 (Sheldrick, 2018)'
_computing_structure_solution    'SHELXT (Sheldrick, 2015)'
_diffrn_ambient_temperature      297(2)
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.987
_diffrn_measurement_device_type  'MAR345 image plate'
_diffrn_measurement_method
;
'60 images, \D\F 3.0\% '
'54 images, \D\F 3.0\% (2nd orientation)'
;
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0195
_diffrn_reflns_av_unetI/netI     0.0163
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.987
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -14
_diffrn_reflns_number            11062
_diffrn_reflns_point_group_measured_fraction_full 0.991
_diffrn_reflns_point_group_measured_fraction_max 0.987
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         26.147
_diffrn_reflns_theta_min         3.262
_diffrn_source                   'Incoatec microfocus source'
_exptl_absorpt_coefficient_mu    0.253
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.71940
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro, Agilent Technologies,
Version 1.171.37.35 (release 13-08-2014 CrysAlis171 .NET)
(compiled Aug 13 2014,18:06:01)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_colour            colourless
_exptl_crystal_density_diffrn    1.389
_exptl_crystal_description       block
_exptl_crystal_F_000             376
_exptl_crystal_size_max          0.40
_exptl_crystal_size_mid          0.30
_exptl_crystal_size_min          0.25
_refine_diff_density_max         0.341
_refine_diff_density_min         -0.366
_refine_diff_density_rms         0.041
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.048
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     232
_refine_ls_number_reflns         3378
_refine_ls_number_restraints     5
_refine_ls_restrained_S_all      1.048
_refine_ls_R_factor_all          0.0438
_refine_ls_R_factor_gt           0.0405
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0456P)^2^+0.4248P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1019
_refine_ls_wR_factor_ref         0.1045
_reflns_Friedel_coverage         0.000
_reflns_number_gt                3113
_reflns_number_total             3378
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            d3ce00226h2.cif
_cod_data_source_block           alex_fl177
_cod_depositor_comments
'Adding full bibliography for 7246740--7246756.cif.'
_cod_database_code               7246744
_shelx_shelxl_version_number     2018/3
_shelx_res_checksum              36483